O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a navegar o site, você aceita o uso de cookies. Leia nosso Contrato do Usuário e nossa Política de Privacidade.
O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a utilizar o site, você aceita o uso de cookies. Leia nossa Política de Privacidade e nosso Contrato do Usuário para obter mais detalhes.
Customer Bulletin 0611 Insulant Impact on Corrosion in Steel Piping Applications Below 32F
Corrosion is defined by the National Association of Corrosion Engineers as “the deterioration of a material, usually a metal, by reaction with its environment.” Corrosion under insulation (CUI) is not a distinct form of corrosion; rather it refers to the location where pipe wall material deterioration is occurring—underneath the insulation material and on the external surfaces of piping. CUI (and the corrosion of metal jackets and banding which is not addressed herein) is a recognized problem that must be addressed by designers, specifiers, and end-users. CUI can occur under any type of thermal insulation. The type of corrosion will depend on the metallurgy of the pipe as well as the mix of corrosive elements - - understanding that corrosive elements can be introduced during pipe production, pipe shipping/storage, installation, insulation contact, process liquid contact, weather, or other environmental influences.
Customer Bulletin 0611 Insulant Impact on Corrosion in Steel Piping Applications Below 32F
Page 1 of 7 CUSTOMER BULLETIN 0611 Insulant Impact on Corrosion in Steel Piping Applications Below 32°FBACKGROUNDCorrosion is defined by the National Association of Corrosion Engineers as “the deterioration ofa material, usually a metal, by reaction with its environment.” Corrosion under insulation (CUI) isnot a distinct form of corrosion; rather it refers to the location where pipe wall materialdeterioration is occurring—underneath the insulation material and on the external surfaces ofpiping. CUI (and the corrosion of metal jackets and banding which is not addressed herein) is arecognized problem that must be addressed by designers, specifiers, and end-users. CUI canoccur under any type of thermal insulation. The type of corrosion will depend on the metallurgyof the pipe as well as the mix of corrosive elements - - understanding that corrosive elementscan be introduced during pipe production, pipe shipping/storage, installation, insulation contact,process liquid contact, weather, or other environmental influences.Focusing on CUI, the three most common types of CUI include oxidation (rusting), stresscorrosion cracking (SCC), and pitting. Yet there are also several specialized types of CUI suchas formicary corrosion1 of copper which in general are not associated with insulated refrigerantsystems and therefore not addressed herein. Metals vary considerably in their susceptibility tovarious types of corrosion.PURPOSEThe purpose of this Customer Bulletin is to provide general information on the causes of CUI insteel pipe, which insulants in general terms may be best for low temperature applications, andhow to avoid of CUI in steel piping systems operating at service temperatures below 32°F.We also discuss how corrosion differs between the two common types of steel2 used in suchpiping systems. To keep it simple, we define carbon steel as steel with less than 10.5%chromium, and stainless steel3 as a steel with a minimum of 10.5% chromium content by weight.1 Formicary (“ants-nest) corrosion may best be described as micro-pitting most common in refrigeration grade copper tubing inHVAC systems although other forms of attack, similar in appearance, have been observed in other alloys. Although poorlyunderstood, attack has been attributed to the growing use of synthetic lubricating oils that were introduced as refrigerant fluidschanged, or to vaporous species derived from the immediate surroundings, including volatiles from process fluids.2 We define “Steel” as an alloy that consists mostly of iron and has a carbon content between 0.2% and 2.1% by weight.3 Refer to http://www.corrosionist.com/Stainless_Steel_grades.htm.CB 0611 June 2011
Page 2 of 7There are of course many types and grades of both carbon and stainless steels, with varyingdegrees of susceptibility to various corrosion processes.SUMMARYToo often, discussions of CUI focus only on the insulation, rather than on the broader spectrumof factors that will more likely be the cause of any CUI. At temperatures below 32F, thelikelihood of any form of CUI is remote. Yet the majority of mechanical systems spend sometime above 32F, such as during outages, so the extent to which an insulant may contribute toCUI must be considered. There are several premises to keep in mind: 1. CUI can in fact occur under any insulant - - some more likely than others a. Insulants with higher Water Absorption and Water Vapor Transmission exacerbate CUI b. Insulants with higher leachable chlorides (or fluorides) can exacerbate CUI (yet such ions must be leachable at the actual temperature presents, and the temperature must be above 32F!) c. CUI is time and temperature dependent 2. CUI can be prevented from occurring by following basic guidelines: - Pre-design identification of environmental factors that could exacerbate CUI, such as rain, acid rain, humidity, “salt air”, wash-down water/chemicals, sprinkler systems, fire control systems, etc.); - Pipe/component design using appropriate metallurgy for the conditions, and control of metallurgy during construction (e.g. welding; pickling/heat treating; avoidance of dissimilar metals in contact; etc.); - Proper specification and application of any pipe coatings; - Proper selection and installation of insulation system materials (insulant, vapor barriers, jackets, mastics, etc.); o This includes compliance with the guidelines of the manufacturers of the various insulation system components as well as the procedures established by a qualified insulation engineer, including for example, keeping the insulation and pipe surfaces dry during the installation process. o Zero-perm vapor barriers can eliminate moisture penetration from the environment. - Operational diligence, including such action as avoidance of excessive impingement of water on pipe during wash-downs, periodic inspection for corrosion, and properCB 0611 June 2011
Page 3 of 7 replacement of the insulation and insulation components after mechanical repairs or inspection.Dyplast is not a piping system designer, so cannot provide credible advice on the overall designof a piping system. We thus focus on insulant selection in the next subsection, and on somegeneral information on corrosion in the remainder of the document - - so the involved partiesmay better understand the issues and thus better able to communicate with system designers,engineers, and contractors. Insulant Selection Selection of the optimal insulant material is first driven by the long term thermal performance of the insulant, just as the first priority of the piping is to ensure mechanical integrity of the process. Corrosion mitigation must inevitably be a secondary concern, unless the pipe system is likely to be exposed to a chemically intense environment, such as an acid regeneration plant in a steel mill with frequent leaks. In such an environment, cellular glass may be the only insulant that could withstand the chemical onslaught, assuming the chemicals do not include hydrogen fluoride, hydrofluoric acid, or related compounds. As explained in Customer Bulletin 0411, polyisocyanurate (particularly Dyplast’s ISO-C1) is inevitably the optimal selection in the vast majority of piping applications with operating temperatures below 32°F. Polyiso’s thermal conductivity combined with its moisture resistance characteristics result in energy savings and process control advantages that far outweigh any concern over corrosion. The additional good news is that ISO-C1 polyiso is low in leachable chloride. At the low temperatures typical of a polyiso installation, CUI is highly unlikely. In systems where there is frequent cycling above 32F, pipe coatings4 can further mitigate any risk of CUI.CORROSION OF STEEL: GENERALWhile dramatically different in nature, the corrosion through oxidation, SCC, and pitting eachshare one common requirement - - moisture. The corrosion of metals is an electrochemicalprocess. That is, there is an electrical circuit where the exchange of electrons (electricity) is4 Typical industry practice is to apply an epoxy primer in the following circumstances: 1) for 300 series stainless steel systemsoperating in a temperature range between 140°F and 300°F or if in a cycling temperature service where the service temperature isbetween 140° and 300°F for more than 20% of the time; and 2) for carbon steel piping operating at a service temperature between32°F and 300°F or in cycling temperature service where the service temperature is between 32°F and 300°F for more than 20%of the time shall be at a minimum primer coated with an epoxy coating. Coating manufacturers should be consulted forappropriate coating materials and application methods for the operating temperature range of the equipment.CB 0611 June 2011
Page 4 of 7conducted by chemical reactions in part of the circuit. These chemical reactions occur at thesurface of the metal exposed to the electrolyte.Water in the form of liquid or vapor must be present at the surface of the metal for corrosion tooccur. Therefore, anything that can be done to prevent moisture (rain, wash-down water,sprinkler systems, condensation, etc.) from reaching the metal surface will help preventcorrosion from occurring. Selecting an insulant with both low water absorption and water vaportransmission, and properly installing a zero-perm vapor barrier with a protective jacket is anappropriate approach in addition to minimizing the external presence of water.The presence of leachable chloride or certain other elements has been found to exacerbatecorrosion. Too often the search for the source of such ions has been centered incorrectly on theinsulation system components, rather than an external environmental factor which is more oftenthe cause.Chemical exposure is the final major environmental element affecting CUI. Acids and acidgases, hydrochloric acid, sulfuric acid, strong bases (caustics), and salts are aggressivecorrosive agents and will both cause and accelerate CUI. The complexity of addressing thereaction of various metals to corrosion by chemicals is beyond the scope of this CustomerBulletin.OXIDATIONOxidation (or simply rusting) is sometimes referred to as uniform corrosion, and is one of themost common mechanisms for corrosion of carbon steel pipe; oxidation does not occur onstainless steel. Oxidation of carbon steel involves four requisites: 1. High temperature 2. Moisture 3. Oxygen 4. Concentration of corrosive ionsIt is an inescapable fact that iron in the presence of oxygen and water is thermodynamicallyunstable with respect to its oxides. Because oxidation corrosion is an electrolytic process, thepresence of an electrolyte is required. This should not be taken to mean that the steel surfacemust be awash in water; a very thin adsorbed film of water is all that is required.Oxidation on carbon steel pipe can occur between 32°F and 300°F; the “optimum” temperaturerange for aggressive corrosion seems to be between 200°F and 240°F5. In this range, there is5 “Is There a Cure for Corrosion Under Insulation?” Michael Lettich, National Insulation Association,http://www.insulation.org/articles/article.cfm?id=IO051101CB 0611 June 2011
Page 5 of 7plenty of heat energy but not enough heat to efficiently evaporate moisture before it contacts theequipment surface. Corrosion rates can double for every 18°F rise in temperature6.At the service temperatures considered in this paper (below freezing point of water), thetemperature should be insufficient to precipitate corrosion even if water, oxygen, and chlorideions are present. Yet, virtually all piping systems spend some time at ambient temperatures,such as during shutdowns for maintenance. Thus there must still be an exerted effort tominimize moisture and the presence of chloride or other environmental contributors or catalystsAn insulation engineer should be consulted when a carbon steel mechanical system cycles intoservice temperatures between 32°F and 300°F for more than 20% of the time. Typical practicein such circumstance is to apply an epoxy coating, or equivalent.PITTING (OR CREVICE) CORROSIONPitting corrosion is a broad term for corrosion that either begins within pits (non-uniformities) inthe pipe surface, or causes pits. Pipe failure can occur if a pit fully penetrates the pipe wall.Pitting can occur in both carbon steel and stainless steel pipes, although it is more commonlyassociated with stainless steels. Pitting is often considered to be more dangerous than uniformcorrosion damage because it is more difficult to detect, predict and design against.Generally, pitting on pipe exteriors can be associated with: - Localized chemical or mechanical damage to the protective oxide films in carbon steel; o chemistry factors such as acidic rain or high concentrations of chloride (as in salt air that has penetrated the insulation system, or indeed from a poorly selected insulant itself in certain circumstances) can cause breakdown of a passive film; and/or - The presence of non-uniformities in the metal structure of the component (e.g. nonmetallic inclusions); and/or - Localized damage to the protective chromium oxide layer on stainless steel (such as at manganese sulfide inclusions on the steel surface) caused by: o chloride or chlorine-containing ions o bromides (fluorides and iodides are not aggressive) o cupric, ferric and mercuric ions (such ions may act in concert with chloride to promote pitting without dissolved O2) [or may indeed prevent pitting in a phosphoric acid environment (e.g. it’s complicated)];6 Mechanical Integrity and Carbon Steel Refrigerant Piping, Daniel J. Dettmers and Douglas T. Reindl, ASHRAE Journal,October 2007CB 0611 June 2011
Page 6 of 7 o thiosulphate ions (S2O3) may also promote pitting.Metals that are susceptible to uniform corrosion (e.g. carbon steel) do not tend to suffer frompitting. Thus, carbon steel will corrode uniformly in sea water, while stainless steel will pit. Anaddition of about 2% of molybdenum increases pitting resistance of stainless steels.Note that crevice corrosion takes place where physical crevices are present, such as at the jointbetween two overlapping sheets of stainless steel, in the crevice between a stainless steelflange and a non-metallic gasket or under surface deposits.STRESS CORROSION CRACKINGSCC is the initiation and propagation of micro-cracks caused by the combined effects of tensilestress coupled with direct surface contact with an enabling chemical7. The stress can beexternally applied, thermal, or residual from the manufacturing process. This stress, coupledwith a susceptible material and environment, causes small cracks inherent or formed in thematerial to propagate - - thereby relieving the material’s stress. If the stress level is low, thecracks will self-limit (stop propagating) prior to fully penetrating the pipe wall. If the stress level ishigh, the cracks have the potential to propagate completely through the entire wall thickness,resulting in a leak.Contrary to conventional wisdom, Stress Corrosion Cracking (SCC) can occur in carbon steelsas well as stainless steels. Yet SCC in carbon steel pipes is unusual on the exterior of the pipesince it requires exposure to either hydroxides, nitrates, carbonate, bicarbonates, liquidammonia, or CO/CO2/H2O at very low temperatures. SCC in carbon steel is more of a concernon the inside the pipe in certain ammonia refrigerant applications/conditions where oxygen maybe present.The most common form of SCC in mechanical systems within the temperature rangesaddressed in this document is Chloride Stress Corrosion of stainless steel pipe, which involvesfour requisites: 1. High temperature 2. Chloride (or fluoride or similar) ions 3. Moisture (dissolved oxygen) 4. Metal is under tensile stressChloride SCC can occur between 140°F and 300°F for 300 series stainless steel. The"optimum" temperature range for aggressive corrosion on 300 series stainless steel seems to7 American Society of Materials International. 2003. ASMI Handbook Volume 13a, Corrosion: Fundamentals, Testing, andProtection, “Selecting Materials to Prevent or Control Corrosion.”CB 0611 June 2011
Page 7 of 7be between 200°F and 240°F. Chloride SCC is most commonly overcome by using a duplexstainless steel, such as 2205, or a grade with a higher nickel content, such as a 6% Mo materialor high-nickel alloys like Alloy 825 (N08825). Ferritic stainless steels are very resistant to SCCbut grades with equivalent pitting resistance to the austenitic grades have other majordrawbacks.CB 0611 June 2011